gellan gum injectable hydrogels for cartilage tissue
Embed Size (px)
Gellan Gum Injectable Hydrogelsfor Cartilage Tissue Engineering Applications:
In Vitro Studies and Preliminary In Vivo Evaluation
Joao T. Oliveira, Ph.D.,1,2 Tırcia C. Santos, B.Sc.,1,2 Luıs Martins, B.Sc.,3 Ricardo Picciochi, B.Sc.,1,2
Alexandra P. Marques, Ph.D.,1,2 Antonio G. Castro, Ph.D.,3 Nuno M. Neves, Ph.D.,1,2
Joao F. Mano, Ph.D.,1,2 and Rui L. Reis, Ph.D.1,2
Gellan gum is a polysaccharide that we have previously proposed for applications in the cartilage tissueengineering field. In this work, gellan gum hydrogels were tested for their ability to be used as injectable systemsusing simple processing methods, able to deliver and maintain chondrocytes by in situ gelation, and support cellviability and production of extracellular matrix (ECM). Rheological measurements determined that the sol–geltransition occurred near the body temperature at 398C, upon temperature decrease, in approximately 20 s. Gellangum discs shows a storage compression modulus of around 80 kPa at a frequency of 1 Hz by dynamic me-chanical analysis. Human articular chondrocytes were encapsulated in the gels, cultured in vitro for total periodsof 56 days, and analyzed for cell viability and ECM production. Calcein AM staining showed that cell kept viableafter 14 days and the histological analysis and real-time quantitative polymerase chain reaction revealed thathyaline-like cartilage ECM was synthesized. Finally, the in vivo performance of the gellan gum hydrogels, interms of induced inflammatory reaction and integration into the host tissue, was evaluated by subcutaneousimplantation in Balb=c mice for 21 days. Histological analysis showed a residual fibrotic capsule at the end of theexperiments. Dynamic mechanical analysis revealed that the gels were stable throughout the experiments whileevidencing a tendency for decreasing mechanical properties, which was consistent with weight measurements.Altogether, the results demonstrate the adequacy of gellan gum hydrogels processed by simple methods fornoninvasive injectable applications toward the formation of a functional cartilage tissue-engineered constructand originally report the preliminary response of a living organism to the subcutaneous implantation of thegellan gum hydrogels. These are the two novel features of this work.
Cartilage is a tissue with relatively low or no turnover,both at cellular and molecular level, which leads to
difficulties in its repair and regeneration once traumatized.The extracellular matrix (ECM) that is responsible for thefunctionality of the tissue has to be maintained by scarcelydistributed chondrocytes, demanding a great anabolic ca-pacity of these cells. Various therapeutic approaches thathave no active biologics were involved, such as arthroscopy,debridement, laser abrasion, drilling, and microfracture.1–3
They involve mostly mechanical techniques that remove theaffected tissue and seek to stimulate the formation of healthytissue. Since the outcomes of these interventions are fre-
quently not satisfactory, namely in terms of functional tissuerecovery, alternative solutions for these problems are beingexplored.1,4,5 Brittberg et al.6 performed autologous chon-drocyte transplantation in 1994 by injecting expandedchondrocytes into cartilage defects subsequently coveredwith a sutured periosteal flap. Although the results weresuccessful in some cases, the percentage of failure led theresearchers to pursue other lines of study, including the useof biomaterials and cells combined with bioactive agents intissue engineering strategies. Several biomaterials, from ei-ther natural or synthetic origin, or combinations of bothtypes, have been proposed as supports for cell developmentand tissue formation in cartilage tissue engineering. Theseinclude alginate, hyaluronic acid, collagen, fibrin, chitosan,
13B’s Research Group—Biomaterials, Biodegradables, and Biomimetics, Department of Polymer Engineering, Headquarters of theEuropean Institute of Excellence on Tissue Engineering and Regenerative Medicine, University of Minho, Guimaraes, Portugal.
2PT Associated Laboratory, IBB—Institute for Biotechnology and Bioengineering, Guimaraes, Portugal.3Life and Health Sciences Research Institute (ICVS), School of Health Sciences, University of Minho, Braga, Portugal.
TISSUE ENGINEERING: Part AVolume 16, Number 1, 2010ª Mary Ann Liebert, Inc.DOI: 10.1089=ten.tea.2009.0117
polyglycolic acid, or polyethylene oxide.7–10 Not only thetype of material is important for the overall performance ofthe constructs but also its processing methodologies and theapplication routes employed. Hydrogels, and especiallyin situ injectable systems, have been gaining a wider interestfor cartilage regeneration applications.11–15 They can be usedin a minimally invasive manner by injecting into the defectarea, normally involve nonharsh methods and reagents,possess the ability to adopt the shape of the defect therebyfacilitating integration, and may be optimized for sol–geltransition to occur near body temperature while encapsu-lating cells and=or bioactive agents of interest.
Gellan gum is a new biomaterial recently proposed fortissue engineering applications,16 namely for cartilage re-generation.17,18 In addition to the above mentioned advan-tages of other injectable systems, gellan gum possess otherfeatures that may place it as a potential candidate for theclinical regeneration of cartilaginous tissues. Gellan gum is alinear anionic polysaccharide composed of repeating units ofglucose, glucuronic acid, and rhamnose.19,20 It exists in theacetylated form, which is the initial raw material, and thedeacetylated form, which is the most commonly used.21,22
Both form thermoreversible gels with differences in me-chanical properties from soft and elastic for the acetylatedform, to hard and brittle for the fully deacetylated polysac-charide which opens interesting prospects for the generationof multifunctional structures.22,23 Gellan gum is noncytotoxicand can be easily processed without the use of harsh re-agents into transparent gels that are resistant to heat and acidstress.24,25 Its gelation is ionotropic as in other polysaccha-rides, like alginate or carrageenan, and therefore the presenceof cations is necessary for the formation of a stable hydrogelstructure. Upon temperature decrease of a gellan gum solu-tion, the transition of a thermally reversible coil to a double-helix chain occurs and is followed by a self-assemblingmechanism that forms oriented bundles. These link them-selves through untwined polysaccharide chain regions cul-minating in the formation of a stable gel.26 The quantity andchemical nature of cations present in solution greatly affectsgellan gum gelation; divalent cations promote a more effi-cient gelation than monovalent cations.26–28 Gellan gum gelsare commonly used in the food industry as thickening agentsor stabilizers.29 In the biomedical field, most applications aresuggested for drug delivery approaches.30–32 Its use in car-tilage tissue engineering was pioneered by our group, andthe application for other soft tissues is currently under study.
In this work, gellan gum hydrogels were used as encap-sulation agents and tissue engineering supports for humanarticular chondrocytes. Gellan gum properties were opti-mized and characterized so that they could be used as in-jectable systems in minimally invasive procedures usingsimple processing methodologies, being this one innovativefeature of this work. Gellan gum with encapsulated humanarticular chondrocytes systems were tested in vitro for peri-ods of up to 56 days of culture. Cell viability and ECMformation and deposition were evaluated by molecular andhistological techniques. A preliminary in vivo evaluationof the gellan gum hydrogels was also performed uponsubcutaneous implantation in Balb=c mice for total periodsof up to 21 days. The obtained results showed the suitabilityof gellan gum hydrogels for injectable applications and in situcell delivery, suggesting a potential application in the future
toward the formation of functional tissue-engineeredcartilage.
Materials and Methods
Cone-plate rheometry was conducted for gellan gum hy-drogels to assess their rheological behavior as function oftemperature and time. For this purpose, gellan gum (G1910;Sigma-Aldrich, St. Louis, MO) powder was mixed at roomtemperature with distilled water at a concentration of 1%(w=v) under constant stirring. The solution was heated to908C and kept at this temperature for 30 min. Afterward,CaCl2 was added to the gellan gum solution at a concen-tration of 0.03% (w=v), and rheological measurements wereperformed using a controlled stress cone-plate rheometer(Reometer Reologica; StressTech, Lund, Sweden). For eachmeasurement, a volume of 2 mL of the gellan gum solutionwas placed in the bottom plate of the rheometer and kept at aconstant temperature of 708C. The polymer solution wasallowed to stabilize for 1 min before starting the experiments.Measurements were performed by decreasing the tempera-ture from 708C to 258C (at a cooling rate of �68C=min) andapplying a constant shear stress of 0.1 Pa. Temperature, time,shear rate, and viscosity were constantly measured. The totalnumber of repeats was five (n¼ 5), and confidence intervalswere estimated with a confidence level of 99%.
Dynamic mechanical analysis
Dynamic mechanical analysis (DMA) was conducted tocharacterize the mechanical behavior of gellan gum hydrogeldiscs. The samples were prepared using a methodologypreviously described elsewhere.25 Gellan gum 1% (w=v)discs (Ø 6� 0.01�5.5� 0.46 mm height) were subjected tocompression cycles of increasing frequencies ranging from 0.1to 10 Hz with constant amplitude displacements of 0.1 mmusing a Tritec 2000 DMA (Triton Technology, Nottingham-shire, United Kingdom). Storage and loss modulus weremeasured, and experiments were conducted at room tem-perature. The total number of discs per assay were five(n¼ 5). The described values for the compression moduluswere collected at a frequency of 1 Hz. Statistical analysis wasperformed using confidence intervals based on the experi-mental results, with a confidence level of 99%.
Human articular chondrocytes isolation and expansion
Human articular cartilage was harvested from the femoralhead and condyles of adult patients (40–65 years) undergo-ing knee arthroplasty surgery. This was performed withinthe scope of a protocol established with the Hospital de S.Marcos, Braga, Portugal, approved by its Ethical Committeeand upon patient informed consent. Chondrocytes wereisolated by enzymatic digestion; in detail, the human artic-ular cartilage, free from all surrounding tissue, was placed ina Petri dish containing sterile phosphate-buffered saline(PBS) and cut into square slices of 5 mm and thickness be-tween 2 and 3 mm. The pieces were washed in sterile PBS,immersed in 20 mL of trypsin–ethylenediaminetetraaceticacid solution, and incubated for 30 min at 378C under agi-tation. Trypsin was removed and the tissue pieces washedwith basic Dulbecco’s modified Eagle’s medium (Sigma-
344 OLIVEIRA ET AL.
Aldrich). Then 20 mL of sterile collagenase type II solution(2 mg=mL) (Sigma-Aldrich) in basic medium was added, andthe mixture was incubated for approximately 12 h at 378Cunder agitation. The digested tissue and cell suspension so-lution was centrifuged at 200 g for 7 min and the supernatantdiscarded. The cell pellet was washed with PBS and centri-fuged again under the same conditions. Cells were againcentrifuged, the supernatant removed, and resuspended inexpansion medium consisting of Dulbecco’s modified Eagle’smedium (Sigma-Aldrich, MO, USA), containing 10 mM [4-(2-hydroxyethyl)-1-piperazineethanesulfonic acid] (HEPES)buffer pH 7.4, 10,000 units=mL penicillin=10,000mg=mLstreptomycin, 20 mM L-alanyl glutamine, 1� minimum es-sential medium (MEM) nonessential amino acids, and 10%(v=v) fetal bovine serum (Biochrom, Berlin, Germany; heatinactivated), supplemented with 10 ng=mL basic fibroblastgrowth factor (PeproTech, London, United Kingdom). Hu-man articular chondrocytes were plated onto tissue cultureflasks and incubated at 378C in a humidified atmosphere of5% CO2 in air for expansion.33
Encapsulation of human articular chondrocytesin gellan gum hydrogels and in vitro culturing
Human articular chondrocytes were expanded and encap-sulated at passage 1 in gellan gum hydrogels using the fol-lowing procedure. Gellan gum powder was mixed with steriledistilled water under constant stirring at room temperature toobtain a final concentration of 1% (w=v). The solution wasprogressively heated to 908C and kept at this temperature for20–30 min. A sterile CaCl2 solution was added to obtain a finalconcentration of 0.03% (w=v). The temperature was progres-sively decreased to 428C and stabilized at this value for pos-terior use always under constant stirring. Human articularchondrocytes were detached by trypsinization, mixed withexpansion medium, and centrifuged at 200 g for 7 min. Thesupernatant was removed, and the cells were resuspended inwarm sterile PBS solution, counted using an hemocytometer,and finally centrifuged at 200 g for 7 min. The supernatant wasdiscarded and the cells pellet kept at the bottom of the falcontube. The gellan gum 1% (w=v) with CaCl2 0.03% (w=v) so-lution was added to the pellet of cells and the mixture re-suspended for complete homogenization of the cells within thematrix. Gellan gum discs containing 8�106 cells=mL humanarticular chondrocytes were produced by casting this mixtureinto sterile cylindrical polystyrene moulds, allowing it to restat room temperature for 1–2 min to form a solid gel. Discs of Ø6� 0.01�5.5� 0.46 mm height were cut using a borer. Thediscs were cultured in the expansion medium for 7 days whichwas afterward replaced by differentiation medium for 49 days.The differentiation medium was prepared by replacing thebasic fibroblast growth factor in the expansion medium withinsulin (1mg=mL) and ascorbic acid (50mg=mL) (Sigma-Aldrich). The culture medium was changed every 3–4 days.
Cell viability: Calcein AM staining
The viability of chondrocytes after 14 days of culture wasassessed using calcein AM staining. Calcein AM (C3099;Invitrogen Corporation, Carlsbad, CA) assay is a fluores-cence-based method for assessing cell viability and cyto-toxicity in which the reagent is retained in cells that have an
intact cell membrane. Briefly, a calcein AM solution of1=1000 was prepared in culture medium. After the end ofeach time point, one disc of gellan gum with encapsulatedhuman articular chondrocytes was collected from the cul-turing plates and incubated in the calcein AM solution for15–30 min at 378C and afterward washed in sterile PBS. 40,6-diamidino-2-phenylindole (DAPI) (Sigma-Aldrich, MO,USA), a fluorescent stain that binds strongly to DNA, wasused for counterstaining. The samples were observed underfluorescent microscopy (Zeiss HAL 100=HBO 100; AxiocamMRc5, Oberkochen, Germany).
Histology (hematoxylin–eosin, Alcian blue, Safranin-O)
Histological analysis was performed with hematoxylin–eosin (H&E), Alcian blue, and Safranin-O staining on 4 mmthickness sections of the cell-scaffold constructs collected atdifferent periods of culture. The samples were fixed in glu-taraldehyde 2.5% (v=v), for 30–40 min at 48C and washed inPBS. Histological processing was performed using Tecnhovit7100� (Heraeus Kulzer, Hanau, Germany) following thecommercial procedure. Sections were cut using a microtomeLeica RM2155 (Leica Microsystems, Nusslock, Germany).H&E staining was performed using automatic processor(Leica Auto Stainer XL) according to the in-house method-ology (Leica TP1020-1; Leica MicroSystems). Histologicalstaining with Alcian blue and Safranin-O was performedusing standard histological methods. The slides were after-ward washed three times in distilled water, quickly dehy-drated through 95% and 100% ethanol, and then cleared inHistoclear� (National Diagnostics, Atlanta, GA) and mountedusing Microscopy Entellan� (Merck, Rahway, NJ) for obser-vation.
Real-time polymerase chain reaction(Sox9, collagen type I, collagen type II, aggrecan)
Samples were collected at defined time periods, quicklyfrozen in liquid nitrogen, and stored at �808C until theanalysis was performed. RNA was extracted using TRIzol�
(Invitrogen Corporation) according to the provided technicaldatasheet. Briefly, three samples of each condition weregrinded and mechanically homogenized with a mortar andpestle in TRIzol reagent, each condition being performed induplicate. Afterward, chloroform was added and the samplescentrifuged to establish a three-phase composition in the tube.The aqueous phase was collected and put in a new tube whereisopropanol was added. The samples were centrifuged,the supernatant discarded and the pellet washed with 75%ethanol. After a final centrifugation the samples were allowedto air dry, and suspended in ultrapure water for posterioranalysis. The amount of isolated RNA and A260=280 ratiowas determined using Nanodrop ND-1000 Spectrophoto-meter (NanoDrop Technologies, Wilmington, DE). After thesedeterminations, 1mg of RNA of each sample was reversetranscribed into cDNA using the IScript� cDNA synthesis kit(Bio-Rad Laboratories, Hercules, CA) in a MJ Mini� PersonalThermal Cycler (Bio-Rad Laboratories). Cartilage-relatedmarkers were chosen to evaluate the chondrogenic phenotypeof the cultured systems. These included Sox9, collagen type I,collagen type II, and aggrecan, using GAPDH as the house-keeping gene for normalization. The expression of each genewas normalized to the GAPDH value in that sample. The
GELLAN GUM INJECTABLE HYDROGELS FOR CARTILAGE TISSUE ENGINEERING 345
relative gene expression quantification was performed usingthe 2�DDCt (Livak) method,34 considering that
2�DDCt¼normalized expression ratio
All the primer sequences were generated using Primer3�software35 and acquired from MWG Biotech� (Ebersberg,Germany). More details can be found in Table 1. Real-timepolymerase chain reaction (PCR) was performed using an MJMini Personal Thermal Cycler (Bio-Rad Laboratories, CA,USA) machine and SYBR Green IQ� Supermix (Bio-RadLaboratories, CA, USA) to detect amplification variations. Theanalysis of the results was performed with MJ OpticonMonitor 3.1 software (Bio-Rad Laboratories).
Subcutaneous implantationin mice—histology and DMA
Gellan gum discs were prepared under sterile conditionsfollowing a methodology previously described.25 Gellan gum1% (w=v) (Ø 6� 0.01 mm�5.5� 0.46 mm height) discs weresubcutaneously implanted in the dorsal part of the Balb=cmice (2–3 months with an average weight of 20 g) duringperiods of up to 21 days. Six female mice were used (two foreach period of implantation). Each animal was anaesthetizedwith a mixture of 5:1 Imalgene� 1000 (Merial, Toulouse,France) and Domitor� (Orion Corporation, Espoo, Finland)(1.25 mg per mouse and 25 mg per mouse, respectively) pre-pared in physiological serum. Under surgical sterile condi-tions, two medial and ventral incisions (approximately0.7 cm) containing the subcutis and the panniculus carnosus(skin smooth muscle) were performed in the dorsum of themice. Craniolateral oriented pockets (two per incision) weresubcutaneously created by blunt dissection. Into these pock-ets, the gellan gum discs were inserted (four discs per animal),and the panniculus carnosus and the skin were carefully su-tured. The animals were kept with food and water ad libitumduring all the time of implantation. After predetermined timeperiods, each test animal was sacrificed, and the implantedscaffolds and respective surrounding tissue were explantedfrom each animal. These were subjected to macroscopic ob-servation and processed for histological analysis to evaluatethe induced inflammatory response and integration into thehost tissue. Briefly, the explanted samples were fixed withformalin solution, dehydrated through ethanol solutions, andembedded in paraffin. Sections with 4 mm thickness of thegellan gum structure and surrounding tissue interface werestained with H&E using automatic coloring equipment, aspreviously described in the ‘‘Histology (hematoxylin–eosin,Alcian blue, Safranin-O Section)’’ section. DMA was alsoperformed using the procedure previously described in the‘‘Dynamic mechanical analysis’’ section.
Rheological measurements were performed mainly todetermine the temperature range at which the sol–gel tran-sition occurred and the time-scale for gelling as these areimportant parameters to look into when the material is ex-pected to be applied as an injectable system and as a cellencapsulating agent. The sol–gel transition temperature wasobserved around 398C (39.4� 0.168C) (Fig. 1). This enablesthe solution to be injected into the organism and gelate at thedefect site once it stabilizes at the body temperature. More-over, the low viscosity of the solution before gelation allowscells to be efficiently mixed and homogeneously dispersedwithin the carrier before the application. Regarding thetime-scale for gelling, it is possible to observe from the graphin Figure 2 that it is approximately 20 s. The results obtainedfor both temperature and time of gelation are critical to dem-onstrate the concept of using gellan gum hydrogels as inject-able systems for minimally invasive surgical proceduresin vivo. A gellan gum solution can be kept above the sol–geltransition maintaining a low viscosity that enables cells orbioactive agents of interest to be homogeneously dispersed.Upon lowering the temperature, the gel forms entrappingthe cells in its matrix in a rather efficient way.
The viscoelastic characterization of the gellan gum hy-drogels was performed using DMA. This technique alsogives important information regarding the mechanical per-formance that these hydrogels may have once implanted
Table 1. Primers Used for Real-Time Polymerase Chain Reaction Evaluation
of Human Articular Chondrocytes Gene Expression
Gene Accession number Left primer Right primer
Sox9 NM_000346 TTGAGCCTTAAAACGGTGCT CTGGTGTTCTGAGAGGCACACollagen type I NM_000089 CTGCAAGAACAGCATTGCAT GGCGTGATGGCTTATTTGTTCollagen type II NM_001844 TCACGTACACTGCCCTGAAG TGCAACGGATTGTGTTGTTTAggrecan NM_001135 ACAGCTGGGGACATTAGTGG GTGGAATGCAGAGGTGGTTTGAPDH NM_002046 GAGTCAACGGATTTGGTCGT TTGATTTTGGAGGGATCTCG
FIG. 1. Rheological measurements of gellan gum solutionsshowing the relation temperature–viscosity and time–viscosity. The sol–gel transition is noticeable by the change inviscosity present in the graph around 398C with an extent oftime for gelation of approximately 20 s.
346 OLIVEIRA ET AL.
in vivo. Gellan gum hydrogels were analyzed in the wet statethroughout a physiological relevant frequency range. Storage(elastic) and loss (viscous) components of the complex mod-ulus were determined and are shown in Figure 2. The storagemodulus (E0) is about one order of magnitude higher thanthe loss modulus (E0 0) which clearly reveals the elastic natureof these gels. It also possesses some damping capability thatmay be useful to dissipate cyclic mechanical energy that isimposed in an implantation scenario. Although some in-crease in E0 is observed for increasing frequencies, the elasticproperties of the hydrogel biomaterial, as compared with theviscous component, are quite stable. An increase in E@ isobserved from 0.6 to 10 Hz, suggesting a higher dissipationcapability of gellan gum hydrogels at higher frequencies. Ata frequency of 1 Hz, the compression modulus of the gelswas estimated to be of 78.6� 2.3 kPa. In fact, although thisvalue does not mimic the mechanical properties found inhuman articular cartilage,36 it is higher or within the range ofvalues found for other hydrogels used in similar cartilageregenerative approaches.8,37
Cell viability and histological analysis
Calcein AM coupled with DAPI fluorescence staining wasconducted to confirm the chondrocyte viability. Calcein AMpenetrates the cell membrane of living cells, being subse-quently hydrolyzed to a cell membrane–impermeable greenfluorescent calcein by esterases present in viable cells. DAPIis a fluorescent stain that binds strongly to DNA. By cou-pling these two agents, viable cells are presented with greencytoplasm and blue nuclei. Results from samples collectedafter 14 days of culture are presented on Figure 3 showingviable human chondrocytes inside the hydrogels. The ma-jority of the cells were positive for calcein and DAPI, whichindicates a dominance of viable cells. These results show thatboth the gellan gum hydrogel is not cytotoxic and that thetemperature cycle used to promote the sol–gel transitiondoes not affect the cell viability.
Histological analysis of samples taken after 56 days ofculture was performed using H&E for regular morphological
cellular analysis, Alcian blue, and Safranin-O that arecommonly used for staining ECM proteoglycans (glycos-aminoglycans). H&E-stained slides (Fig. 4A, B) show anhomogeneous chondrocyte distribution throughout the gel-lan gum hydrogel matrix. Representative images of the de-position of proteoglycans (glycosaminoglycans) within thegellan gum matrix, commonly found in native articularcartilage ECM, can be found in Figure 4C and D. A positivestaining in some pericellular areas of newly formed cellclusters was observed. An improvement in the nature of thestaining that evolved from a more orthochromatic in theinitial periods of culture (data not shown) to a more pro-nounced metachromatic staining in the latter periods wasalso noticed. This effect was more evident in the regionswhere cell clusters formed in comparison to individualchondrocytes.
Real-time PCR (Sox9, collagen type I,collagen type II, aggrecan)
Real-time PCR is frequently used to amplify and simul-taneously quantify a specific sequence in a DNA sample.This technique was used to assess the expression profile ofdifferent molecules associated with hyaline cartilage ECMand thereby evaluate the nature and type of matrix that isbeing formed. Quantitative data may be obtained on geneexpression and variations that are occurring (upregulation ordownregulation) in comparison to a housekeeping gene.Sox9, collagens type I and II, and aggrecan are common ECMconstituents, and their expression pattern from 14 to 56 daysof culture was assessed (Fig. 5). GAPDH was chosen as thereference housekeeping gene since most of the studies pre-sented on chondrocytes gene expression use this standardand therefore the results can be analyzed in a comparativeway. The cycle threshold (Ct) value for each sample wasdetermined only when the exponential phase of amplifica-tion was reached. In each sample, the Ct value was nor-malized to the Ct value of the reference gene (GAPDH).Collagen type II and aggrecan are considered to be the two
FIG. 2. Mechanical properties evaluation of gellan gumdiscs using dynamic mechanical analysis. The tests wereperformed in intervals of 0.1–15 Hz in hydrated samples.
FIG. 3. Calcein AM=40,6-diamidino-2-phenylindole viabil-ity staining of human articular chondrocytes encapsulated ingellan gum hydrogels at 14 days of culture. Color imagesavailable online at www.liebertonline.com=ten.
GELLAN GUM INJECTABLE HYDROGELS FOR CARTILAGE TISSUE ENGINEERING 347
major and most important constituents of hyaline cartilageECM since the functionality of this tissue relies mostly on thepresence of these components. Both collagen type II andaggrecan experienced a significant increase of approximately400-fold and 35-fold, respectively, from 14 to 56 days ofculture in the gellan gum with encapsulated human chon-drocytes hybrid systems. Collagen type I was not detectedafter 56 days and Sox9 was downregulated to values close tozero from 14 to 56 days.
In vivo tests: Histology, mechanical analysis,and weight measurements
The initial response of a living organism to any kind ofimplanted biomaterial is absolutely necessary before pro-ceeding to further tissue engineering studies. For this, thesubcutaneous implantation of a biomaterial and the subse-quent evaluation of the extent of the provoked inflammatoryresponse is a common first screening methodology. As a wayto confirm the adequacy of the developed hydrogels to beput through further screening, gellan gum discs were sub-cutaneously implanted in the back of Balb=c mice for periodsof up to 21 days. Upon explantation, no evident macroscopicchanges of the discs and surrounding tissues were observedafter this period and the discs maintained its structural
FIG. 4. Histological analysis of sections of gellan gum with human articular chondrocytes after culturing. Hematoxylin–eosin (A, B—after 2 and 56 days of culture, respectively) was used for general cell morphology and distribution, whereasAlcian blue (C) and Safranin-O (D) were performed for proteoglycans (glycosaminoglycans) detection. Color images avail-able online at www.liebertonline.com=ten.
FIG. 5. Graphical representation of the real-time semi-quantitative polymerase chain reaction analysis for collagentype I, collagen type II, aggrecan, and Sox9 based on themRNA produced by the encapsulated human articularchondrocytes after 14 and 56 days of culture. Statisticalanalysis through the various time points (p> 0.05) was per-formed using a two-sample t-test assuming unequal var-iances for n¼ 3, a¼ 0.05. Statistically significant differencesare marked with an asterisk (*).
348 OLIVEIRA ET AL.
integrity. Histological analysis of the explanted samples,stained with H&E, showed good integration within thesurrounding host tissue. In terms of inflammatory response–associated cells, the normal presence of neutrophils wasobserved at 7 days of implantation (Fig. 6A, B). This cellpopulation revealed a progressive decrease along theimplantation time, almost inexistent at 14 days (Fig. 6C, D).Additionally, a thin and residual fibrotic capsule (Fig. 6E, F)and the infiltration of some phagocytic cells (Fig. 6F, arrow)were evident by the end of 21 days. DMA performed on thehydrogel samples at different periods of explantation re-
vealed no statistically significant differences between thesamples, although a slight decrease tendency in the com-pressive modulus was noticed (Fig. 7). In terms of weightmeasurements, which can be an indicator of biodegradationof gellan gum hydrogels, a statistical difference was ob-served after 21 days of implantation. Although the weightsof the samples at different time points did not present rele-vant alterations, a statistically significant decrease was no-ticed after 21 days when compared with nonimplantedgellan gum gel discs and gel discs with 14 days of implan-tation (Fig. 8).
FIG. 7. Storage and loss modulus at 1 Hz obtained fromcompression dynamic mechanical tests of gellan gum discsafter subcutaneous implantation in Balb=c mice. Statisticalanalysis was performed using a two-sample t-test assumingunequal variances for n¼ 5, a¼ 0.05 and revealed no differ-ence through the various time points ( p> 0.05).
FIG. 8. Weight measurements of gellan gum discs aftersubcutaneous implantation in Balb=c mice. Statistical analy-sis revealed a significant difference (*) in gellan discs im-planted for 21 days when compared with no implant and 14days of implantation. Statistical analysis through the varioustime points ( p> 0.05) was performed using a two-samplet-test assuming unequal variances for n¼ 5, a¼ 0.05.
FIG. 6. Histological analysis showing two different magnifications of sections of gellan gum after 7 (A, B), 14 (C, D), and21 (E, F) days of implantation. The images evidenced a good integration with the surrounding tissue and the progressivereduction of the fibrotic capsule that was almost unnoticed after 21 days. The arrow (F) indicates the infiltration of phagocyticcells. Color images available online at www.liebertonline.com=ten.
GELLAN GUM INJECTABLE HYDROGELS FOR CARTILAGE TISSUE ENGINEERING 349
The use of hydrogels in cartilage regeneration is consid-ered to be a promising strategy due to some intrinsic featuresthat they frequently exhibit. Most of them can be applied asminimally invasive systems that are able to deliver cellsand=or bioactive agents of interest in situ and to keep them atthe implantation site. The processing under mild conditionscoupled to the use of nonharsh reagents is another positiveaspect. In addition, the gelation in situ enables the formedhydrogel to quickly set its volume and easily adapt to theshape of the defect site, establishing an efficient integrationwith the host tissue.38 Gellan gum is a new biomaterialproposed for cartilage regeneration that exhibits those fea-tures. It can be prepared by simple methods using nonag-gressive reagents and can be combined with cells or bioactiveagents of interest at the body temperature and physiologicalpH. It can be injected under a minimally invasive surgicalintervention and gelate upon temperature stabilization atbody temperature giving rise to an efficient defect filling andcell entrapment system. Another potentially interesting as-pect is the structural unit of gellan gum that includes glu-curonic acid in its composition.19 This monosaccharideresidue possesses a functional carboxylic group that may bemodified to confer improved functionalities to this bioma-terial. One final aspect is the fact that this biomaterial is al-ready used in humans in ophthalmic applications,39 whichmay clearly enable a fast approval by the regulatory bodies.In this work, gellan gum hydrogels were tested for theirability to be used as injectable systems using simple methodsin cartilage repair applications, which may be useful in thefuture in minimally invasive approaches. The injectability ofthis biomaterial was analyzed and confirmed by rheologicalmeasurements. Cone-plate rheology was used to determinethe temperature range and time duration of the sol–geltransition in gellan gum hydrogels. The gellan gum solutionrevealed a consistent increase in viscosity around 408C thatstabilized at approximately 398C, being the temperature atwhich the gelation process is finalized. This analysis alsoprovided data on the time during which this process oc-curred which was shown to be of approximately 20 s. Theinterpretation of both these parameters demonstrates thepotential of these hydrogels to be used as minimally inva-sive injectable systems that are able to deliver and encap-sulate cells and=or bioactive agents to a defect site in thehuman body. In addition, the injectability of gellan gumhydrogels is good since their viscosity before the onset ofgelation is low, enabling the overall mixing and applicationof the gel to be easily conducted. Mechanical propertiestested using DMA retrieved a wet state compression mod-ulus of approximately 80 kPa at a frequency of 1 Hz analyzedin the wet state using a physiologically relevant frequencyrange. The storage modulus (E0) is about one order of mag-nitude higher than the loss modulus (E0 0) which indicates anelastic nature of gellan gum. Some damping capability wasnoticed when analyzing tan d results, which may be con-sidered an advantage for dissipating some cyclic mechanicalenergy that is generated in vivo. This value is fairly goodwhen compared to other hydrogels frequently described inthe literature for cartilage regenerative approaches.8,37
Nonetheless, human cartilage exhibits higher compressive
modulus of approximately one order of magnitude.36 Thisdifference is expected to be compensated by ECM depositionduring the formation of a cartilaginous structure.8 In vitrotests showed that chondrocytes were viable and homoge-neously distributed inside the hydrogels as observed underfluorescence microscopy using calcein AM combined withDAPI and H&E staining. The chondrocytes’ typical round-shaped morphology was confirmed at both initial and long-term culture periods. Cell dispersion throughout the gellangum matrix was quite homogeneous and the cells main-tained normal morphological features and active division tosome extent. Using the calcein AM-DAPI staining it waspossible to observe that the chondrocytes are viable insidethe matrix, although cell division state may somehow belimited due to the physical restrictions of the hydrogel net-work which is a typical feature in similar systems.40 None-theless, it may be that the carbohydrate nature of gellan gum,which contains high glucose content, can be used as a sourceof energy by the cells, thereby progressively giving rise tospaces within the hydrogel matrix and the consequentchondrocyte proliferation. Ongoing work performed by ourgroup on the subcutaneous implantation of gellan gum discsthrough extensive periods has gathered consistent informa-tion that corroborates this hypothesis. Other mechanicalevents associated with cell proliferation may include theformation of microcracks and the propagation of fracturecreating additional spaces for cell growth. Besides cells’viability and distribution, the formation of an adequate ECMis of utmost importance to the performance of the tissue-engineered construct. Active collagen type II and aggrecandeposition contributes to the formation of a functional hya-line-like cartilage-engineered tissue. These are in fact thetwo major ECM molecules responsible for the articular car-tilage mechanical properties; collagen type II confers tensilestrength, and aggrecan is responsible for the compressiveresistance.41 Alcian blue and Safranin-O performed after 56days of culturing on sections of gellan gum with encapsu-lated human articular chondrocytes evidenced glycosami-noglycans deposition in the pericellular regions of most cellclusters. Real-time PCR analysis for Sox9, collagen I, collagenII, and aggrecan strengthened these findings confirming theincreased levels of expression of transcripts from collagentype II and aggrecan from 14 to 56 days. Collagen type II wasupregulated approximately 400-fold and aggrecan approxi-mately 35-fold; no statistically significant variation in Sox9was encountered and no collagen type I was detected. Suchresults clearly show that human articular chondrocytesencapsulated in gellan gum hydrogels were able to deposita hyaline-like ECM, therefore contributing to the formationof a functional tissue-engineered construct. However, thelow expression of Sox9 seems to diverge from this patternsince this factor is apparently associated with the chon-drocyte phenotype maintenance and collagen type II ex-pression, although this is not consensual.42,43 Chondrocytesfrom osteoarthritis cartilage present low levels of Sox9,43 andthe cell source may be a possible explanation for this oc-currence. Also, the dedifferentiation process occurring dur-ing in vitro expansion44 or the existence of some associatedhypertrophy of the chondrocytic cells may be occurring.45
The following step in this study was to evaluate the re-sponse of a host to a first contact with this biomaterial, which
350 OLIVEIRA ET AL.
to our knowledge is for the first time report in this work.Gellan gum discs were subcutaneously implanted in the backof Balb=c mice, and histological analysis was conducted toassess the inflammatory processes associated with the im-plantation, as well as the integration into the host tissue. Anegligent, thin, and residual fibrotic capsule was observedwith no evident polymorphonuclear and mononuclear cellspresent, as well as a good integration with the involvingtissues. It should be mentioned that some phagocytic cellinfiltration (Fig. 6F, arrow) into the hydrogel matrix wasobserved after 21 days, indicating that this might be aprobable scenario in further in vivo studies. One mightspeculate that such an event will enable gellan gum withencapsulated cell systems to efficiently integrate with thehost tissues and establish a functional transition zone at theinterface area, although this must be shown in furtherstudies.
DMA performed on the explants after the defined timeperiods revealed no statistically significant differencesamong the various samples. Weight measurements showedthat although no relevant alterations were detected, a sig-nificant decrease was noticed after 21 days. This may cor-relate with some cell infiltration into the gellan gumhydrogel matrix and possible resorption, as observed inthe histological analysis. In an in vivo scenario where thegellan gum carries encapsulated cells intended to form atissue, the tendency may be the deposition of a cartilage-likeECM along with the possible degradation of the hydrogel.Further studies on this respect will be conducted to under-stand how gellan gum will degrade or will be replaced at theimplantation site by the newly formed tissue. As a summary,this work demonstrates the potential of gellan gum hydro-gels to be used as injectable systems in minimally invasivesurgical procedures for cartilage regeneration. The propertiesof this biomaterial were characterized and shown to becompatible with the application envisaged. The in vitrostudies with clinically relevant cells showed successful hu-man articular chondrocyte viability and ECM formation,culminating with the in vivo reaction evaluation upon im-plantation of the gels in an ectopic site. The overall dataanalysis shows that this injectable system has all the re-quirements to be used for cartilage tissue engineering and itspotential should continue to be assessed by further in vivostudies.
Gellan gum hydrogels were originally proposed and usedin the herein presented studies as injectable systems for celldelivery and support, aimed at cartilage regeneration, usingsimple nonharsh processing methodologies. Gellan gumability to be applied as a minimally invasive system uponinjection and in situ gelation was supported by rheologicalmeasurements. The gels exhibit a low viscosity between 428–418C enabling an efficient and homogeneous mixing of thecells, that can afterwards be injected forming a stable gel withentrapped cells when reaching the body temperature. Gela-tion occurs around 398C in about 20 s. The evaluation of themechanical properties of the hydrogels showed that these arewithin the normal range of other hydrogels used in theseapplications and should be able to adapt to the cartilage en-
vironment. In vitro tests performed with human articularchondrocytes encapsulated in gellan gum hydrogels revealedthat the cells remained viable and produced hyaline-like ECMas observed by the significant increase of collagen type IIand aggrecan after 56 days of culture. Subcutaneous im-plantation of these materials in the back of mice revealedhighly satisfactory results since the histology evidenced in-tegration of the gels within the host tissue with no persistentinflammatory response. The DMA showed that the gelsmaintained their mechanical stability, and weight measure-ments by the end of the experiments reinforced these obser-vations. Taking together all these data, it can be concludedthat gellan gum hydrogels are adequate for injectable appli-cations and in situ cell delivery in cartilage regenerationapproaches. This new biomaterial has generated interestingand promising results that justify its use in further in vivostudies highly benefiting from their ease of processing per-formed under nonharmful conditions to the cells with theability to be injected at the defect site in a minimally invasivemanner. Its ability to be used as an injectable system usingthe described processing methodologies and the prelimi-nary in vivo response performed by the subcutaneous im-plantation in mice are the two major innovations presented inthis work.
J.T. Oliveira would like to acknowledge the PortugueseFoundation for Science and Technology for his grant(SFRH=BD17135=2004). The authors would like to thank thepatients at Hospital de S. Marcos, Braga, Portugal for thedonation of the biological samples, and the medical staff fortheir help and support. The authors would also like to thankthe Institute for Health and Life Sciences, University ofMinho, Braga, Portugal, for allowing the use of their re-search facilities. This work was carried out under the scopeof the European NoE EXPERTISSUES (NMP3-CT-2004–500283) and partially supported by the European ProjectHIPPOCRATES (STRP 505758–1).
No competing financial interests exist.
1. Hunt, S.A., Jazrawi, L.M., and Sherman, O.H. Arthroscopicmanagement of osteoarthritis of the knee. J Am Acad OrthopSurg 10, 356, 2002.
2. Caplan, A.I., Elyaderani, M., Mochizuki, Y., Wakitani, S.,and Goldberg, V.M. Principles of cartilage repair and re-generation. Clin Orthop Relat Res 342, 254, 1997.
3. Cancedda, R., Dozin, B., Giannoni, P., and Quarto, R. Tissueengineering and cell therapy of cartilage and bone. MatrixBiol 22, 81, 2003.
4. Ge, Z., Hu, Y., Heng, B.C., Yang, Z., Ouyang, H., Lee, E.H.,and Cao, T. Osteoarthritis and therapy. Arthritis Rheum 55,
493, 2006.5. Mano, J.F., and Reis, R.L. Osteochondral defects: present
situation and tissue engineering approaches. J Tissue EngRegen Med 1, 261, 2007.
GELLAN GUM INJECTABLE HYDROGELS FOR CARTILAGE TISSUE ENGINEERING 351
6. Brittberg, M., Lindahl, A., Nilsson, A., Ohlsson, C., Isaksson,O., and Peterson, L. Treatment of deep cartilage defects in theknee with autologous chondrocyte transplantation. N Engl JMed 331, 889, 1994.
7. Risbud, M.V., and Sittinger, M. Tissue engineering: ad-vances in in vitro cartilage generation. Trends Biotechnol 20,
351, 2002.8. Tuzlakoglu, K., Alves, C.M., Mano, J.F., and Reis, R.L. Pro-
duction and characterization of chitosan fibers and 3-D fibermesh scaffolds for tissue engineering applications. Macro-mol Biosci 4, 811, 2004.
9. Lee, C.R., Breinan, H.A., Nehrer, S., and Spector, M. Ar-ticular cartilage chondrocytes in type I and type II collagen-GAG matrices exhibit contractile behavior in vitro. TissueEng 6, 555, 2000.
10. Hutmacher, D.W. Scaffolds in tissue engineering bone andcartilage. Biomaterials 21, 2529, 2000.
11. Stile, R.A., Burghardt, W.R., and Healy, K.E. Synthesis andcharacterization of injectable poly(N-isopropylacrylamide)-based hydrogels that support tissue formation in vitro.Macromolecules 32, 7370, 1999.
12. Elisseeff, J., McIntosh, W., Anseth, K., Riley, S., Ragan, P.,and Langer, R. Photoencapsulation of chondrocytes inpoly(ethylene oxide)-based semi-interpenetrating networks.J Biomed Mater Res 51, 164, 2000.
13. Drury, J.L., and Mooney, D.J. Hydrogels for tissue engi-neering: scaffold design variables and applications. Bioma-terials 24, 4337, 2003.
14. Hoemann, C.D., Sun, J., Legare, A., McKee, M.D., andBuschmann, M.D. Tissue engineering of cartilage using aninjectable and adhesive chitosan-based cell-delivery vehicle.Osteoarthritis Cartilage 13, 318, 2005.
15. Schagemann, J.C., Erggelet, C., Chung, H.W., Lahm, A.,Kurz, H., and Mrosek, E.H. Cell-laden and cell-free bio-polymer hydrogel for the treatment of osteochondral defectsin a sheep model. Tissue Eng Part A 15, 75, 2009.
16. Smith, A.M., Shelton, R.M., Perrie, Y., and Harris, J.J. Aninitial evaluation of gellan gum as a material for tissue en-gineering applications. J Biomater Appl 22, 241, 2007.
17. Oliveira, J.T., Picciochi, R., Santos, T.C., Martins, L., Pinto,L.G., Malafaya, P.B., Sousa, R.A., Marques, A.P., Castro,A.G., Mano, J.F., Neves, N.M., and Reis, R.L. Injectablegellan gum hydrogels as supports for cartilage tissue engi-neering applications. Annual Tissue Engineering and Re-generative Medicine International Society—EuropeanChapter Meeting, Mary Ann Liebert Inc., Porto, Portugal,2008, p. OP165.
18. Gong, Y., Wang, C., Lai, R.C., Su, K., Zhang, F., and Wang,D.-a. An improved injectable polysaccharide hydrogel:modified gellan gum for long-term cartilage regenerationin vitro. J Mater Chem 19, 1968, 2009.
19. Jansson, P.-E., Lindberg, B., and Sandford, P.A. Structuralstudies of gellan gum, an extracellular polysaccharideelaborated by Pseudomonas elodea. Carbohydr Res 124, 135,1983.
20. Moorhouse, R., Colegrove, G.T., Sandford, P.A., Baird, J.K.,and Kang, K.S. PS-60: A New Gel-Forming Polysaccharide.Washington, DC: D.A. Brandt, 1981.
21. Rozier, A., Mazuel, C., Grove, J., and Plazonnet, B. Gelri-te(R): a novel, ion-activated, in-situ gelling polymer forophthalmic vehicles. Effect on bioavailability of timolol. IntJ Pharm 57, 163, 1989.
22. Grasdalen, H., and Smidsrod, O. Gelation of gellan gum.Carbohydr Polym 7, 371, 1987.
23. Kang, K.S., and Veeder, G.T. Polysaccharide S-60 and bac-terial fermentation process for its preparation. United StatesPatent 4326053 (1982).
24. Ogawa, E., Takahashi, R., Yajima, H., and Nishinari, K. Ef-fects of molar mass on the coil to helix transition of sodium-type gellan gums in aqueous solutions. Food Hydrocoll 20,
378, 2006.25. Oliveira, J.T., Martins, L., Picciochi, R., Malafaya, P.B., Sousa,
R.A., Neves, N.M., Mano, J.F., and Reis, R.L. Gellan gum: anew biomaterial for cartilage tissue engineering applica-tions, J Biomed Mater Res A, Aug 5, 2009 (Epub ahead ofprint).
26. Quinn, F.X., Hatakeyama, T., Yoshida, H., Takahashi, M.,and Hatakeyama, H. The conformational properties of gel-lan gum hydrogels. Polym Gels Netw 1, 93, 1993.
27. Ogawa, E., Matsuzawa, H., and Iwahashi, M. Conforma-tional transition of gellan gum of sodium, lithium, and po-tassium types in aqueous solutions. Food Hydrocoll 16, 1,2002.
28. Miyoshi, E., Takaya, T., and Nishinari, K. Rheological andthermal studies of gel-sol transition in gellan gum aqueoussolutions. Carbohydr Polym 30, 109, 1996.
29. Mao, R., Tang, J., and Swanson, B.G. Texture properties ofhigh and low acyl mixed gellan gels. Carbohydr Polym 41,
331, 2000.30. Coviello, T., Dentini, M., Rambone, G., Desideri, P., Carafa,
M., Murtas, E., Riccieri, F.M., and Alhaique, F. A novel co-crosslinked polysaccharide: studies for a controlled deliverymatrix. J Control Release 55, 57, 1998.
31. Kubo, W., Miyazaki, S., and Attwood, D. Oral sustaineddelivery of paracetamol from in situ-gelling gellan and so-dium alginate formulations. Int J Pharm 258, 55, 2003.
32. Sanzgiri, Y.D., Maschi, S., Crescenzi, V., Callegaro, L., Topp,E.M., and Stella, V.J. Gellan-based systems for ophthalmicsustained delivery of methylprednisolone. J. Control Release26, 195, 1993.
33. Crawford, A., and Dickinson, S.C. Chondrocyte isolation,expansion, and culture on polymer scaffolds, In: Hollander,A.P., and Hatton, P.V., eds. Methods in molecular biology:Biopolymer methods in tissue engineering. Totowa, NJ:Humana Press Inc., 238, 147, 2004.
34. Livak, K.J., and Schmittgen, T.D. Analysis of relative geneexpression data using real-time quantitative PCR and the2�DDCT method. Methods 25, 402, 2001.
35. Page, D.C., and Lander, E.S. Available at http:==frodo.wi.mit.edu=. 2008.
36. Froimson, M.I., Ratcliffe, A., Gardner, T.R., and Mow, V.C.Differences in patellofemoral joint cartilage material prop-erties and their significance to the etiology of cartilage sur-face fibrillation. Osteoarthritis Cartilage 5, 377, 1997.
37. Nettles, D.L., Vail, T.P., Morgan, M.T., Grinstaff, M.W.,and Setton, L.A. Photocrosslinkable hyaluronan as a scaffoldfor articular cartilage repair. Ann Biomed Eng 32, 391, 2004.
38. Hoffman, A.S. Hydrogels for biomedical applications. AdvDrug Deliv Rev 54, 3, 2002.
39. Dickstein, K., Hapnes, R., and Aarsland, T. Comparison ofaqueous and gellan ophthalmic timolol with placebo on the24-hour heart rate response in patients on treatment forglaucoma. Am J Ophthalmol 132, 626, 2001.
40. Weber, M., Steinert, A., Jork, A., Dimmler, A., Thurmer, F.,Schutze, N., Hendrich, C., and Zimmermann, U. Formationof cartilage matrix proteins by BMP-transfected murinemesenchymal stem cells encapsulated in a novel class ofalginates. Biomaterials 23, 2003, 2002.
352 OLIVEIRA ET AL.
41. Knudson, C.B., and Knudson, W. Cartilage proteoglycans.Semin Cell Dev Biol 12, 69, 2001.
42. Aigner, T., Gebhard, P.M., Schmid, E., Bau, B., Harley, V.,and Poschl, E. SOX9 expression does not correlate with typeII collagen expression in adult articular chondrocytes. MatrixBiol 22, 363, 2003.
43. Tew, S.R., Clegg, P.D., Brew, C.J., Redmond, C.M., andHardingham, T.E. SOX9 transduction of a human chon-drocytic cell line identifies novel genes regulated in primaryhuman chondrocytes and in osteoarthritis. Arthritis Res Ther9, R107, 2007.
44. Lefebvre, V., Li, P., and de Crombrugghe, B. A new longform of Sox5 (L-Sox5), Sox6 and Sox9 are coexpressed inchondrogenesis and cooperatively activate the type II col-lagen gene. Embo J 17, 5718, 1998.
45. Akiyama, H., Chaboissier, M.C., Martin, J.F., Schedl, A., andde Crombrugghe, B. The transcription factor Sox9 has es-sential roles in successive steps of the chondrocyte differ-entiation pathway and is required for expression of Sox5 andSox6. Genes Dev 16, 2813, 2002.
Address correspondence to:Joao T. Oliveira, Ph.D.
3B’s Research Group—Biomaterials, Biodegradablesand Biomimetics
Department of Polymer EngineeringHeadquarters of the European Institute of Excellence on Tissue
Engineering and Regenerative MedicineUniversity of Minho
AveParkZona Industrial da Gandra
S. Claudio do Barco4806-909 Caldas das Taipas
E-mail: [email protected]
Received: February 19, 2009Accepted: August 24, 2009
Online Publication Date: October 7, 2009
GELLAN GUM INJECTABLE HYDROGELS FOR CARTILAGE TISSUE ENGINEERING 353
This article has been cited by:
1. Shiva H. Jahromi, Liam M. Grover, Jennifer Z. Paxton, Alan M. Smith. 2011. Degradation of polysaccharide hydrogels seededwith bone marrow stromal cells. Journal of the Mechanical Behavior of Biomedical Materials . [CrossRef]
2. Haeyeon Lee, Stephanie Fisher, Michael S. Kallos, Christopher J. Hunter. 2011. Optimizing gelling parameters of gellan gumfor fibrocartilage tissue engineering. Journal of Biomedical Materials Research Part B: Applied Biomaterials n/a-n/a. [CrossRef]
3. Daniela F. Coutinho, Shilpa V. Sant, Hyeongho Shin, João T. Oliveira, Manuela E. Gomes, Nuno M. Neves, Ali Khademhosseini,Rui L. Reis. 2010. Modified Gellan Gum hydrogels with tunable physical and mechanical properties. Biomaterials 31:29,7494-7502. [CrossRef]
4. João T. Oliveira, Leandro S. Gardel, Tommaso Rada, Luís Martins, Manuela E. Gomes, Rui L. Reis. 2010. Injectable gellangum hydrogels with autologous cells for the treatment of rabbit articular cartilage defects. Journal of Orthopaedic Research 28:9,1193-1199. [CrossRef]
5. J. T. Oliveira, R. L. Reis. 2010. Polysaccharide-based materials for cartilage tissue engineering applications. Journal of TissueEngineering and Regenerative Medicine n/a-n/a. [CrossRef]
6. J. Silva-Correia, J. M. Oliveira, S. G. Caridade, J. T. Oliveira, R. A. Sousa, J. F. Mano, R. L. Reis. 2010. Gellan gum-basedhydrogels for intervertebral disc tissue-engineering applications. Journal of Tissue Engineering and Regenerative Medicine n/a-n/a.[CrossRef]